2.
38 M. Farle et al.
experiments, see for example [1]), one has to keep in mind that orbital dynam-
ics which couples the spin moment to the crystal lattice is an important ingredient
in spin dynamics. The orbital contribution is often hidden in a so-called effective
spin model [2] or neglected due to its small contribution (<10 %) to the overall
magnetization for example in 3d ferromagnets. In nanoscale structures, however, the
contribution of orbital magnetism to spin dynamics may become important due to the
increased percentage of magnetic moments which are located at surfaces and inter-
faces where they experience a low-symmetry electrostatic potential (crystal ﬁeld)
causing an enhanced orbital magnetic moment. Here, we will restrict our discussion
to the model of effective spins or effective magnetization, respectively.
This chapter is organized as follows. We will begin with a short reminder on at
ﬁrst sight different manifestations of “spin dynamics” in ferromagnetic materials
followed by a short overview of experimental techniques to record ferromagnetic
resonance phenomena in materials with sub-micron dimensions. Magnetoresistive,
microwave resonance, and optical detection schemes will be presented in a more
detailed form in respective sections. This experimental part is preceded by a general
discussion of the current understanding of how a magnetization relaxes to its ground
state after resonant microwave or spin current excitation.
In spin dynamics—like in any other type of time evolution of a physical quantity—
one has to consider the magnetic response in relation to the type (i.e. vector or scalar),
amplitude and energy spectrum of the excitation as well as the relaxation rates and
likely different dissipation channels allowing the stored energy to dissipate to the lat-
tice. A wide energetic range of excitations produced by time varying magnetic ﬁelds
has been investigated in the frequency and time domain of spin dynamics. Depending
on the amplitude of the excitation linear- and non-linear magnetic responses which
are described by the ﬁeld- and frequency-dependent magnetic susceptibility tensor
χ can be monitored. The phenomena can be subdivided into ultrafast magnetization
processes (few tens to hundreds of femtoseconds) and processes evolving on the ps to
ns timescale [3]. We will restrict our discussion to the later, that is resonant processes
at 1 − 100GHz frequencies.
The temperature dependence of the magnetization is governed by the thermally
excited energy spectrum of elementary excitations of the magnetization called spin
waves or magnons [4]—which are always present at ﬁnite temperatures (at 295K
there are app. 1021−1022 cm−3 magnons). Spin waves follow dispersion relations
[5] which depend on crystallographic orientation, size and shape of the ferromagnet
[6, 7]. The dispersion relations for the spin wave vector (q) covering momentum
transfers over the full Brillouin zone and the energy range from µeV to several
tens of meV (Stoner excitations), or that is in wavelength covering the range of
tens of micrometers to nearest neighbor atomic distances, have been conﬁrmed by
experimental techniques like Brillouin Light Scattering (BLS) (see for example [8]),
inelastic neutron scattering and energy loss spectrocopy (see for example [9]).
The term spin dynamics also covers the research areas of thermally induced
“spin ﬂuctuations” and “spin excitations” which for example become visible in the
temperature dependence of the interlayer exchange coupling of two ferromagnetic
layers coupled across a normal metal spacer layer like Cu [10], the temperature
3.
Spin Dynamics in the Time and Frequency Domain 39
dependence of the macroscopic magnetic anisotropy energy density (MAE) or at the
para-ferromagnetic phase transition in form of the so-called critical broadening of
the magnetic resonance linewidth at the Curie temperature (see for example [11]).
A very straight forward way to see the effect of spin excitations is the temperature
dependence of the magnetization at low temperatures (T 3/2 law). As evidenced in
cubic nanoparticles the changes of the magnon excitation spectrum due to conﬁne-
ment are readily reﬂected in a modiﬁed temperature dependence of the macroscopic
magnetization [12]. Also, it has been shown by scanning tunneling spectroscopy that
the lifetime of a localized excited spin state of an Fe atom [13], which is a sensitive
measure of magnetic dipole-dipole and exchange interactions with its local and dis-
tant environment, varies between 50 and 250ns depending on its local coordination.
Available techniques cover the non-linear (large excitation amplitudes) and lin-
ear response regime. In the latter case the exciting microwave power is limited to
a few tens of mW and the precession angle of the magnetization is only a few
degrees. Ideally, only coherent precession of the magnetization is excited, that
is to say we consider dispersion relations in the long spin wavelength (λ) limit
that is 2π/λ = q → 0. The discussion will be restricted to recent advances
in modeling and experimental techniques, since the state of the art of measuring
and modeling magnetization dynamics in conﬁned magnetic structures has been
described up to the year 2006 in three excellent books edited by B. Hillebrands and
K. Ounadjela [14].
In recent years a number of time-resolved techniques have been developed with
the aim to measure and image magnetization dynamics in magnetic micro and nanos-
tructures. The magnetization state is probed using X-rays or light in the visible range.
The contrast mechanism is X-ray magnetic circular dichroism or the magneto-optical
Kerr effect respectively. While X-ray based techniques such a X-ray photoemission
microscopy (XPEEM) or scanning transmission X-ray microscopy (STXM) [15]
can have a spatial resolution as high as 20nm, their time resolution is limited by the
electron bunch length of the synchrotron to about 30 ps, i.e. a few GHz. Brillouin
light scattering (BLS) (see for example [8, 16]) and time resolved Kerr microscopy
(TRMOKE) [17] on the other hand can achieve only a moderate spatial resolution of
200–300nm. The sub picosecond time resolution, however, allows to follow magne-
tization dynamics well into the THz regime [18]. Recent developments also include
element-resolved spectroscopies in alloyed or composite ferromagnetic materials
like X-ray Detected Magnetic Resonance (XDMR) [19] in which X-ray Magnetic
Circular Dichroism (XMCD) [20, 21] can be used to probe the resonant precession
of local magnetization components in a strong microwave pump ﬁeld up to the THz
regime and X-ray Resonant Magnetic Scattering (XRMS) which probes the motion
of the magnetization stroboscopically as a function of time after magnetic ﬁeld pulse
excitation [22, 23].
4.
40 M. Farle et al.
(a) (b)
Fig. 1 a Simpliﬁed scheme showing the relaxation of the magnetization vector after microwave
excitation. Restoring torques according to the Landau-Lifshitz-Gilbert equation are indicated.
b Block diagram of the two most simple relaxation channels after microwave excitation. q is
the wavevector of a magnon. Adapted from [24]
2 Energy Dissipation Channels for Reversal and Relaxation
of the Magnetization
In general, one can say that the understanding of spin dynamics in nanomagnets
requires a detailed knowledge of the precessional motion of the magnetization vec-
tor, involving the conditions for spin wave generation and dispersions and differ-
ent relaxation channels after excitation. It involves various research areas in theory
as well as in experiment (resonance, spin-torque, spin-injection, magnetic rever-
sal, non-linear dynamics) to interpret the different modes of magnetic damping,
relaxation and magnon scattering. Topics which will be touched upon involve linear
versusnon-linearprocesses,spin-spinversusspin-orbitdrivenmechanisms,frequency-
versus time-domain measurements, ground state magnetism versus magnetism in an
excited state. For all these mechanisms characteristic differences between metallic
and insulating ferromagnets exist. Another interesting problem is the classiﬁcation
in dissipative and non-dissipative mechanisms in regard to the energy of the spin
system.
We start very simply with the discussion of the relaxation of the magnetization by
considering the phenomenological model of a precessing macroscopic magnetization
of a ferromagnetic material Fig.1a. In this model one considers a homogeneous
magnetization which is the vectorial sum of initially collinear magnetic moments.
The Larmor frequency of the precessional motion is well described by the Landau-
Lifshitz equation from which the static magnetic properties appearing in the equation
can be determined by angular- and frequency dependent FMR measurements. As
discussed in [25] the resonance frequency ω is calculated by:
ω
μB g/
2
=
1
M2 sin2 (θ)
∂2 F
∂θ2
∂2 F
∂φ2
−
∂2 F
∂θ∂φ
2
(1)
5.
Spin Dynamics in the Time and Frequency Domain 41
where ω is the microwave frequency, g—the g-factor, φ and θ—azimuthal and polar
equilibrium angles of the vector of magnetization M. Different forms of the free
energy density functional F can be used. The following exemplary expression is
valid for the geometry of an ultrathin ﬁlm [25]:
F = −μ0M · Hext − μ0 M H⊥ cos2
θ + K
||
2 sin2
θ sin2
φ − φK2
+ K4 sin2
θ −
K4
8
(7 + cos 4φ) sin4
θ (2)
that includes the Zeeman term, the perpendicular anisotropy ﬁeld H⊥, the in-plane
uniaxial anisotropy K
||
2 with its easy axis deﬁned by the in-plane angle φK2 and
the cubic magneto-crystalline anisotropy K4. The anisotropy ﬁelds Ki /M can be
obtained with an accuracy of <1%. The error of the anisotropy constants is domi-
nated by the uncertainty of the saturation magnetization of ≤10%, evaluated from
magnetometry measurements.
This analysis determines only the eigenfrequency of the uniform precession of the
macroscopic magnetization, that is only the magnons with q = 0. If one considers
regionally non-collinear or in other words in time and space varying (out-of-phase)
excited states, one can derive dispersion relations ω(q) for magnons which in the
case of a thin ﬁlm are for example given by [26] :
ω = γ μ0 H + μ0 Ms 1 −
1 − e−qd
qd
sin2
φq + Dq2
+ HMAE1
× μ0(H + H⊥) − μ0 Ms 1 −
1 − e−qd
qd
+ Dq2
+ HMAE2
1/2
(3)
ω is a function not only of the wave vector q, but also of the external magnetic ﬁeld H
and sample parameters such as saturation magnetization Ms, effective perpendicular
ﬁeld H⊥, spin wave stiffness D, ﬁlm thickness d, the spectroscopic splitting factor
γ = μB g/ , and parameters HMAE1 and HMAE2, which are functions of very small
anisotropyﬁelds.Here,φq describestheanglebetweenthemagnetizationandthespin
wave vector. As explained in detail in Ref.[26] φq is very small, so that sin φq ≈ 0.
The dynamic response of the magnetization is described by the equation of motion
given by Landau and Lifshitz and the damping term suggested by Gilbert.
dM
dt
= −γ (M × μ0Heff) +
α
M
M ×
dM
dt
(4)
where M is the magnetization. The damping parameter α in SI units is related to the
commonly used Gilbert damping factor G in CGS units by α = G4π/μ0 Mγ .
In a recent review by Fähnle et al. (see [3] and references therein) it was sum-
marized that this phenomenological picture can be also understood in terms of
electron-magnon scattering. It was calculated that the dominant contributions to the
dissipative part of the dynamics in metallic ferromagnets arise from the creation of
6.
42 M. Farle et al.
electron-hole pairs and from their subsequent relaxation by spin-dependent scatter-
ing processes which transfer angular momentum to the lattice. Effective ﬁeld theories
(generalized breathing and bubbling Fermi-surface models) have been developed [3]
which show that the Landau-Lifshitz-Gilbert equation of motion should be extended
for the description of ultrafast magnetization processes, but in general provides an
quantitatively excellent approach for the description of spin dynamics. Recently,
Barsukov et al. [28] established by detailed frequency dependent FMR measurements
and ab initio electronic structure calculations using the fully relativistic Korringa-
Kohn-Rostoker Green’s function method within spin-density-functional theory that
the damping factor α is isotropic and depends on the composition in Fe1−x Six thin
ﬁlms. These ﬁlms show for all compositions 0 < x < 40 a very small composition
dependent anisotropy K4 (Fig.2a). This may explain the observed and calculated
isotropic behavior of α which in general should reﬂect the anisotropy of the orbital
magnetic moment μl. As already pointed out by Kambersky (see [29] and references
therein), for magnetic metallic systems two processes Eq.(5) for the relaxation of the
net magnetization dominate the Gilbert damping factor G. Both ordinary and spin-
ﬂip scattering processes depend on the density of states at the Fermi level N(EF )
and on the electron scattering time τ. They are directly proportional to the square of
the deviation of the g-factor from its free spin-value [29]:
Spin − ﬂip − scattering : G =
γ
2
2
N(EF )(g − 2)2
/τ (5)
Ordinary − scattering : G =
γ
2
2
N(EF )λ2
SO(g − 2)2
/τ (6)
Since the magnetic anisotropy energy density is related to the anisotropy of the
orbital magnetic moment δμl and since the g-factor measured in FMR (see for exam-
ple [30]) is a measure of the orbital-to-spin magnetic moment ratio, one could hope
to identify anisotropic Gilbert-type (spin-orbit) damping only in materials with large
magnetic (uniaxial) anisotropy [31]. It must be noted, however, that the identiﬁca-
tion of such a intrinsic anisotropic Gilbert damping may be impossible due to the
presence of the so-called two-magnon scattering which can also cause an angular
dependent relaxation rate.
In a very simple scheme the relaxation channels of the excited magnetization
can be described by the cartoon in Fig.1b which dates back to discussions by
H. Suhl recently reviewed in [32, 33]. The scheme indicates that uniform magnons
with q = 0—that is the uniformly precessing magnetization in Fig.1a—are excited
by microwave (RF) excitation. The uniform magnons can relax either via spin-orbit
coupling and phonon-magnon interaction directly to the lattice or by dissipationless
magnon-magnon scattering into non-zero wave vector magnon states followed by
relaxation to the lattice. The intrinsic Gilbert damping path leads to heating of the
lattice which for example can be used to detect magnetic resonance in a nanomagnet
[34]. The other route indicated by the dashed arrow represents an initially dissipation
free channel. Uniform magnons scatter into magnons with q = 0 but with the same
7.
Spin Dynamics in the Time and Frequency Domain 43
(a)
(b)
(c)
Fig. 2 Magnetic anisotropy energy and magnetic damping constant of Fe1−x Six as a function of
Si concentration. a Magneto-crystalline anisotropy constant K4. Red dots show experimental data
extracted from combined SQuID and FMR measurements on thin ﬁlms grown on MgO(001). Error
bars are 10% due to the error in determining the magnetic volume. Black dots show the results of
the DFT calculations for Fe-Si bulk-systems at 0K. b Gilbert-damping parameter: black squares
are results of the DFT calculation showing a minimum at x ∼= 20 %. Red dots are experimental data
obtained by frequency-dependent FMR measurements. Dashed line is a guide to the eye according
to the theoretical data. c Average spin magnetic moment μs and electron density of states at the
Fermi edge n(EF ). The dependence on Si concentration correlates with the dependence of the
Gilbert parameter. From [27]
energy ω as the q = 0 state. Such a process is only feasible if the momentum transfer
q = 0 → q = 0 is negligible and degenerate states in energy are available (compare
Fig.1b). The Suhl (q = 0) magnons eventually lose their energy to the lattice. In the
literature these two principally different relaxation channels are either referred to as
intrinsic versus extrinsinc or Gilbert-type versus dissipation free channels. They are
associated with different relaxation times T1 and T2 or in other words a longitudinal
and transverse relaxation time as can be described by the Bloch-Bloembergen form
of the Landau-Lifshitz equation:
8.
44 M. Farle et al.
dmz
dt
= −γ (m × μ0Heff)z −
mz − MS
T1
(7)
dmx,y
dt
= −γ (m × μ0Heff)x,y −
mx,y − MS
T2
(8)
In regard to the simple relaxation scheme of Fig.1a one realizes that the dissipa-
tion free relaxation channel (dashed arrow) in the Scheme 1b results in a temporary
decrease of the length of the magnetization vector associated with the transverse
relaxation time T2 or in other words a dephasing of the coherently precessing mag-
netic moments. A pure Gilbert type of relaxation would not lead to a change of the
magnitude of the magnetization, and the tip of the vector would spiral along the sur-
face of a sphere to its ground state. Finally, by annihilation of the Suhl magnons the
system recovers its full magnetization given by the longitudinal relaxation time T1.
The two-magnon scattering mechanism has been described theoretically by Arias
and Mills [26, 35] based on the linear response theory and experimentally conﬁrmed
by several groups. In a two-magnon process a uniform magnon (q = 0) initially
created in a thin ﬁlm with the magnetization lying in plane is scattered into a non-
uniform state with the same energy and different wave vector q S = 0, as shown
in Fig.3 (straight dotted line). Due to the local nature of this scattering process the
momentum conservation can be violated [36]. In Fig.3 the magnon dispersion for
an ultrathin ﬁlm magnetized in-plane including dipole-dipole interaction is shown.
For the spin wave vector in-plane and parallel to the magnetization (φ = 0 < φC )
the blue dispersion relation is obtained. Energetically degenerate states q S and q 0
exist which can be coupled via the scattering potential FSC AT . Usually, FSC AT is
given by randomly distributed defects in a thin ﬁlm. If the angle φ between the in-
plane direction of the magnetization and the wave vector increases beyond a critical
angle φC , the degeneracy of the q 0 and q S states is lifted, and the two-magnon
scattering process becomes inoperative- allowing a straight forward identiﬁcation in
the experiment.
For applications that require certain relaxation times one wants to control the
relaxation rate while maintaining the desired static magnetic properties of a material
such as its magnetic anisotropy energy density, the saturation magnetization and
interlayer exchange coupling. Some concepts for modifying the local damping in
metallic ferromagnets, which unfortunately involve the risk of altering the static
magnetic properties are:
• Doping with different elements [37–39]
• Ion mixing [40]
• Ion-induced segregation [41]
• Surface patterning of metallic layers by ion implantation [28]
• Formation of a regular defect pattern by oblique deposition in binary alloy ﬁlms
(e.g. Fe3Si [42]).
An interesting possibility to minimize the unwanted changes of the static para-
meters of a ferromagnetic layer is the so-called spin-pumping effect [43]. By adding
9.
Spin Dynamics in the Time and Frequency Domain 45
Fig. 3 Dispersion relation (including dipolar interaction) for magnons in a thin ﬁlm. A number of
uniform (q||0) magnons are annihilated (a−) and a number non-uniform magnons (nS) with q||S = 0
are created (a+). This process is mediated by the scattering ﬁeld FSC AT which couples both magnon
states. The number of uniform magnons (n0) is increased by the microwave excitation and reduced
by relaxation processes like the two-magnon scattering
a non-ferromagnetic metallic layer a spin-sink for a diffusive spin-current gener-
ated by the precessing magnetization after microwave excitation across the ferro-
magnetic/normal metal interface is created. Here, one has to be aware that this is
a non-localized form of magnetic relaxation. The spin current carries away angu-
lar momentum from the ferromagnet into the normal metal where it is dissipated.
Considerable effects have been seen in multilayered structures in which the relative
orientation of two ferromagnetic layers separated by a normal metal layer determines
the magnitude of the additional spin-pumping contribution to the intrinsic Gilbert
damping [44]. The addition of the normal metal layer, however, may also modify
the local crystalline structure by strain relief or creation [45] and thereby modify the
static magnetic parameters like the magnetic anisotropy energy density.
Recently, a new approach for mesoscopically sized magnetic structures has been
suggested based on the control of the two-magnon scattering mechanism. This
approach realizes one possible route to extrinsically inﬂuence the longitudinal relax-
ation time—as indicated by the box of ‘interfering ﬁelds” or scattering potentials for
magnons in Fig.1b. By artiﬁcially designing a periodic potential whose periodicity
is adapted to the dominating magnon excitations the scattering rate can be enhanced
and thereby the extrinsic or longitudinal relaxation time shortened. This is indicated
in Fig.3 by the scattering ﬁeld Fscat .
The analysis of experimental FMR linewidths should at least include four different
contributions ([46] and references therein):
B(ω, ψB) = BGilbert
(ω, ψB) + Bmosaic
(ω, ψB)
+ B2mag
(ω, ψB) Binhom
(9)
10.
46 M. Farle et al.
Here B denotes the peak-to-peak linewidth of the FMR signal. ψB denotes the
two angles θB and φB, the ﬁrst being the polar angle of the external ﬁeld measured
with respect to the ﬁlm normal and the latter the azimuthal angle of B measured with
respect to the in-plane [100]-direction.
The four different contributions to the FMR linewidth of Eq.(9) are:
(i) The Gilbert contribution BGilbert.
In various magnetic systems, the damping can be described by the phenom-
enological Gilbert damping parameter G. If the Gilbert damping represents the
entire intrinsic damping, then it follows from the Landau-Lifshitz-Gilbert equa-
tion of motion that the FMR linewidth should depend linearly on the microwave
frequency [31]. In order to determine G or α, frequency-dependent FMR mea-
surements over a large range of microwave frequencies are needed. Note, that
the linear frequency dependence of FMR linewidth is valid only when the mag-
netization and external magnetic ﬁeld are parallel to each other. Otherwise the
so-called ﬁeld dragging contribution has to be included. If one wants to express
relaxation rates in terms of linewidths, i.e. to convert from frequency-swept to
the ﬁeld-swept linewidth measured by FMR one can use the following conver-
sion:
B(ω, ψB) = γ
d Bres(ω, ψB)
dω
·
ω
γ
. (10)
Here (ω
γ ) is the frequency-swept linewidth written in magnetic ﬁeld units. The
sufﬁx ‘res’ indicates that d Bres(ω, ψB)/dω has to be calculated at the resonance
condition. In Eq.(10) ω is a function of B and ψB(B), therefore Eq.(10) can
be written as
B(ω, ψB) = γ
∂ Bres(ω, ψB ≡ constant)
∂ω
·
ω
γ
+ γ
∂ Bres(ω ≡ constant, ψB)
∂ψB
·
dψB
dω
·
ω
γ
. (11)
The second term in Eq.(11) is commonly called the ﬁeld-dragging contribution,
because the partial derivative gets large at angles for which the magnetization
M is dragged behind B = μ0H due to magnetic anisotropy effects. Along the
hard and easy axes of magnetization, for which M and µ0 H are parallel, this
dragging contribution vanishes. The Gilbert damping contribution in Eq.(9) is
therefore given by:
BGilbert
(ω, ψB ≡ β) ≈
2
√
3
α
γ
ω
cos β
(12)
11.
Spin Dynamics in the Time and Frequency Domain 47
where β is the angle between the magnetization M and external ﬁeld μ0H. For
the in-plane conﬁguration β = φeq −φH and for the out-of-plane conﬁguration
β = θeq − θH .
(ii) Line broadening due to mosaicity ( Bmosaic).
The second term in Eq.(9) is the so called mosaicity term. It is caused by a
small spread of sample parameters on a very large scale. This variation can be
found in the internal ﬁelds, thickness, or orientation of crystallites within the
sample. The individual regions thus have slightly different resonance ﬁelds. The
overall signal will be a superposition of these local FMR lines yielding a broader
linewidth. We consider the ﬂuctuations of the directions of the anisotropy ﬁelds
by the mosaicity contribution given by:
Bmosaic
(ω, ψB) =
∂ Bres(ω, ψB)
∂φB
φB +
∂ Bres(ω, ψB)
∂θB
θB (13)
where φB and θB represent the average spread of the direction of the easy
axes in the ﬁlm plane and normal to the ﬁlm, respectively. Note that for fre-
quency dependent measurements along the easy and hard axes the partial deriv-
atives are zero and thus the mosaicity contribution vanishes.
(iii) The two-magnon scattering contribution B2mag.
The two-magnon scattering is a process, where the q = 0 magnon excited by
FMR scatters into degenerate states of magnons having wave vectors q = 0.
This process requires that the spin-wave dispersion allows for degenerate states,
and that there are scattering centers in the sample. The geometrical separation of
the scattering centers is connected to the extension of the ﬁnal magnon states in
real space. If long wavelength spin-waves are involved in the relaxation process,
defects of the order of several 100nm rather than atomic defects act as scattering
centers.Theexistenceoftwo-magnonscatteringhasbeendemonstratedinmany
systems of ferrites.
The linewidth B2mag caused by the two-magnon scattering mechanism is a
measure of the scattering rate of the uniform (q = 0) magnons into other spin-wave
modes (q = 0). For a homogenously magnetized thin ﬁlm, B2mag can be expressed
as [47]:
B2mag
(ω, ψB) ∝
xi
xi f (φB − φ xi )
× arcsin
⎛
⎝ ω2 + (ω0/2)2 − ω0/2
ω2 + (ω0/2)2 + ω0/2
⎞
⎠ U θeq − θc (14)
with ω0 = γ μ0 Meff = γ (μ0 M − 2K2⊥/M) and μ0 Meff being the effective magne-
tization that consists of μ0 M and the intrinsic out-of-plane anisotropy ﬁeld 2K2⊥/M.
μ0 Meff can be determined by analyzing the angle dependent FMR resonance ﬁeld.
The factor xi denotes the strength of the two-magnon scattering along the
12.
48 M. Farle et al.
principal in-plane crystallographic direction xi . This parameter will be ﬁtted to
the experimental data. The f (φH − φ xi )-term allows for the two-magnon contri-
bution to depend on the in-plane direction of μ0H relative to the principal in-plane
crystallographic directions xi given by the angles φ xi . An angle dependent two-
magnon scattering may occur when the scattering centers are not isotropic within the
sample. In the case that the centers are given by lattice defects, the angular depen-
dence should reﬂect this lattice symmetry. In the case that different contributions
of two-magnon scattering along the principal crystallographic directions xi occur,
one has to sum up these contributions weighted by their angular dependence given
by f . The step function U θeq − θc in Eq.(14) is equal to 1 for θeq > θc and zero
for θeq < θc. It is used to describe the ‘switching off’ of the two-magnon scattering
at a critical out-of-plane angle of the magnetization. Theoretically, it is shown that in
oblique conﬁguration, when the magnetization is tipped out of the ﬁlm plane, ﬁnite
wave vector modes are degenerate with the FMR mode for |θeq| > |θc| = 45◦. Thus
the two-magnon scattering should be operative in this regime of the tipping angle,
but it should shut off for |θeq| < |θc| = 45◦. It has been shown that the angular
dependence of the two-magnon scattering can be approximated by a step function.
3 Ferromagnetic Resonance Detection in the Frequency Domain
3.1 Cavity Ferromagnetic Resonance
For macroscopic bulk samples Ferromagnetic Resonance has been measured using
standard microwave technology based on microwave cavities working at ﬁxed fre-
quencies in a narrow band of about 1, 2, 4, 9, 26.5, 35 and 75GHz (so called L-,S-,
C-, X-, K-, Q- and W-band). The magnetic ﬁeld part of the microwave ﬁeld is perpen-
dicular with respect to the external magnetic ﬁeld which can be swept from 0 to 2.3
Tesla using electromagnets. The appearance of the resonance is observed by moni-
toring the reﬂected rectiﬁed microwave power from the microwave cavity. Setups for
measurements of the Ferromagnetic Resonance (FMR) (or Electron Spin Resonance
(ESR) for paramagnetic molecules) in ultrahigh vacuum have been developed (see
[25] and references therein). For example, the temperature dependence of the mag-
netic properties of ferromagnetic monolayers under ultrahigh vacuum conditions,
surface states (dangling bonds) at silica surfaces, and sub-monolayer coverages of
paramagnetic molecules/atoms at low temperatures has been successfully analyzed
[1, 48]. Standard cavity based spectrometers offer a detection limit of 1010 to 1014
paramagnetic moments with spin S = 1/2 provided the resonance linewidth is nar-
rower than 10mT [49]. This corresponds to a coverage of paramagnetic atoms or
molecules on a cm2 surface of 10−4 to 1 monolayer. Recently, the “cavity” concept
was successfully miniaturized to the micron scale [50]. Due to the increased ﬁlling
factor different spin wave modes in a single permalloy micron-sized stripe could be
detected and quantitatively compared to the results of micromagnetic simulations.
13.
Spin Dynamics in the Time and Frequency Domain 49
This new approach offers currently an ultimate sensitivity of 106 magnetic moments
corresponding to a nanoparticle of less than 100nm diameter.
In the FMR experiment the presence of different relaxation channels (Fig.1b) as
discussed in the previous section is identiﬁed by the frequency dependence of the
linewidth ( B) of the resonant spin precession [45, 46, 51]: The Gilbert damping
exhibits a linear frequency dependence, whereas the two-magnon scattering follows
the curved arcsin-like Eq.(14) behavior [26]. Although non-monotonous linewidth
behavior had been considered for disordered polycrystalline systems previously [36],
only recently (see for example references in [35, 52, 53]) systematic investigations
on how to unambiguously identify and eventually control the two magnon relaxation
mechanism have been published. Here we will discuss two examples beginning with
the effects of a network of defects created in Fe3Si ultrathin ﬁlms by oblique deposi-
tion of the constituents. In the following chapter the frequency-selective enhancement
of the magnetic relaxation rate by designing the periodicity of the defect structure
will be demonstrated.
In [42] oblique angle deposition of Si during the deposition of 40nm thick Fe3Si
epitaxial thin ﬁlms on MgO(001) was used to create a network of defects with
a preferential orientation. It could be demonstrated that this procedure created an
effective scattering ﬁeld for two-magnon scattering with 2-fold symmetry, whose
preferential direction can be chosen by the deposition angle during ﬁlm growth and
whose scattering rate = 0.2GHz is comparable with the Gilbert damping of Fe3Si
in X-band. In Fig.4 the experimental data which were extensively discussed and
compared to theory in [42] are reproduced. By the uniaxial symmetry of the oblique
deposition process an additional twofold contribution to the two-magnon scattering
process can be controlled in magnitude and orientation by creating chemical disorder
with a symmetry axis along any given in-plane direction and thus independently of
the fourfold contribution from the network of unavoidable defects reﬂecting the
cubic symmetry of the crystal lattice. The Si is deposited under an oblique angle of
approximately 15◦ with respect to the ﬁlm normal and the projection of the incident
Si stream on the ﬁlm plane is referred to as axis β (Fig.4a). Such growth conditions
are known to provoke so-called shadow effects.
Figure4b shows the in-plane angular dependence of the resonance ﬁeld Bres of a
40nm thick ﬁlm measured at 9.3GHz and 295K (Sample #2). Using the saturation
magnetization MS = 0.96(8)106 A/m measured by SQuID magnetometry, the effec-
tive perpendicular anisotropy ﬁeld is B⊥ ≈ 1T and the in-plane magnetocrystalline
anisotropy constant K 4 ≈ (3.3 ↔ 4.3)103 J/m3 can be calculated from the ﬁt (solid
line) to the data (red circles). The in-plane uniaxial anisotropy constant is small
and amounts to K 2(0.1 ↔ 0.5)103 J/m3. Except for this small uniaxial anisotropy,
a comparison with anisotropy values of the samples grown by non-oblique depo-
sition reveals that the modiﬁed growth conditions do not considerably change the
static magnetic parameters. However, there is a correlation of the in-plane uniaxial
anisotropy K 2 and the sample preparation. The hard axis of K 2 is aligned parallel
to the in-plane projection β of the Si ﬂow. Indeed, stripelike defects caused by the
shadow effect are known to induce such magnetic anisotropy in thin ﬁlms by means
14.
50 M. Farle et al.
Fig. 4 a Sketch of the ﬁlm
deposition geometry. Oblique
deposition of Si causes stripe-
like defects with the symmetry
axis perpendicular to the
projection of the Si-ﬂow β.
b–d: 40nm Fe3Si/MgO(001)
FMR data at 9.3GHz. b
In-plane angular dependence
of FMR resonance ﬁelds,
revealing the 4-fold crystalline
anisotropy K 4 and the small
uniaxial anisotropy K 2.
FMR linewidth: c The native
4-fold contribution 4- f old
caused by crystalline defects
is superimposed by the 2-fold
contribution 2- f old . The
maximum of the latter one
is parallel to the hard axis of
the uniaxial anisotropy and
corresponds to the in-plane
projection of the Si-ﬂow:
φ2- f old = φuniax = β.
d Linewidth of the sample #1,
for which the axis β was set
close to the [110] direction.
From [42]
(b)
(a)
(c)
(d)
of the dipolar interactions among the defects. The low value of K 2 suggests a low
density of these defects.
The FMR linewidth Bpp allows to identify the relaxation processes in the sam-
ple. In Fig.4c the experimental linewidth (black line) is shown as a function of
in-plane angle φB of the magnetic ﬁeld. This in-plane angular dependence exhibits
a behavior remarkably different from that of a regular ﬁlm grown with a non-tilted
Si evaporator [46]. While it has the typical fourfold symmetry of Fe3Si/MgO(001)
ﬁlms, one also ﬁnds an additional twofold contribution superimposed. The latter
15.
Spin Dynamics in the Time and Frequency Domain 51
Table 1 Static and dynamic magnetic parameters (at X-band) of Fe3Si/MgO(001) prepared under
different growth conditions
Sample, Si deposition and K
||
4 K
||
2
max
100
max
110
max
twof old φtwof old
ﬁlm thickness (103 J/m3) (103 J/m3) (107 Hz) (107 Hz) (107 Hz) (deg)
#1 Oblique, 40nm 4.0 0.2 51 13 20 49
#2 Oblique, 40nm 3.8 0.5 58 30 33 74
#3 Oblique, 40nm, not annealed 2.7 0.25 269 95 33 74
#5 normal, 40nm (from Ref. [46]) 3.3 − 53 26 − −
Error bar of anisotropy constants: <10%, of max
ζ : ∼30%, of max
twof old : <10%, and of φtwof old :
<5◦
turns out to be of the same order of magnitude as the fourfold contribution and the
Gilbert contribution. The simulation (red line) of the experimental Bpp is the same
as of the afore mentioned contributions to the FMR linewidth whose ﬁtted angu-
lar dependences are shown by the green (fourfold two-magnon, extrinsic), brown
(twofold extrinsic),blue(inh mosaicity,extrinsic)andyellowgreen(isotropicGilbert,
intrinsic) solid lines. The corresponding equations have been given in [42] and are not
reproduced here. This angular dependence can be compared with the one of a nearly
identical sample (#1) which was deposited with a change of the plane of incidence
of the oblique Si stream. The angular dependence of Bpp reveals the change of the
plane of incidence from β#2 to β#1 (Fig.4d). The calculated ﬁt parameters for the
magnetic anisotropy constants and two-fold and four-fold scattering rates are given
in Table1 in comparison to a non-annealed ﬁlm and a ﬁlm deposited with normal
incidence of Si.
As shown in the Table1, the modiﬁed growth conditions do also not affect the
4-fold two-magnon scattering process f our f old. Its intensity is comparable with
results presented in [46]. The effective size of the rectangular, randomly located
defects assumed for the ﬁtting procedure lies in the range of few hundreds of
nanometers—being plausible for the distance between crystalline defects in this sys-
tem. Comparing the results of samples #1 and #3 reveals, that despite the modiﬁed
growth the f our f old intensity can be decreased by means of sample annealing.
3.2 Non-Cavity Approaches to FMR Detection
In this section we will brieﬂy refer the reader to a selection of detection schemes of
Ferromagnetic Resonance in the frequency domain which do not require the classical
microwave cavity approach. The following list gives a few examples of such schemes.
• Ferromagnetic Resonance Force Microscopy [54]
• Photothermally Modulated Ferromagnetic Resonance (PM-FMR) for locally
resolved and depth dependent measurements [55]
16.
52 M. Farle et al.
• Scanning Thermal Microscopy Ferromagnetic Resonance (SThM-FMR) [56],
offering a lateral resolution of <100nm and a sensitivity of 106 spins
• High-sensitivity broadband microwave spectroscopy with small non resonant coils
[57]
• Broadband bolometric detection of resonant absorption in ferromagnetic nanopar-
ticles [34]
• Broadband resonance detection of paramagnetic inclusions in weak links of
Josephson junctions [58]
• Micro-resonators at ﬁxed frequencies [50])
• Stripline and shorted wave guide based FMR techniques (see [51] and references
therein).
Each of these schemes has certain advantages for speciﬁc materials and appli-
cations. Some of these techniques allow to sweep the frequency in a range of 1 to
10GHz or even higher microwave frequencies, while in others the magnetic ﬁeld is
swept at constant microwave frequency. Also, one has to consider if one needs to
characterize materials under ultrahigh vacuum (UHV) conditions, as a function of
temperature, frequency and/or applied magnetic ﬁeld strength/angle (see for exam-
ple [25]). It is worthwhile to note that Kalarickal et al. [51] showed experimentally
for three methods that frequency or ﬁeld swept techniques yield the same FMR
linewidth.
In the following we present a recent experimental result (Fig.5) showing the
possibility of manipulating the relaxation rate of permalloy ﬁlms by introducing an
artiﬁcial periodic scattering ﬁeld FSC AT . As described in detail in [28] a well-deﬁned
periodically modulated surface magnetization (scattering ﬁeld FSC AT , Fig.3) of a
permalloy ﬁlm was prepared by low-dosage Cr implantation along stripes of width
s0 and separation s1. In regard to the schematics in Fig.3 one may expect to see
characteristic changes in the relaxation rates due to extrinsic (two magnon) damp-
ing contributions. According to the theory developed by Landeros and Mills [59]
increases of the FMR linewidth as a function of frequency are expected at character-
istic spin wave vectors qp reﬂecting the periodicity of the magnetization modulation.
In Fig.5 the ﬁrst experimental observation [28] of this effect is shown. Using a newly
developed shortened-coaxial-waveguide setup [60], which is UHV compatible, the
FMR linewidth was determined in a quasi-continuous frequency range of 2 – 26GHz.
In Fig.5a the experimental frequency dependence of the linewidth for the magnetic
ﬁeld applied parallel to the stripes with periodicity l = s1 + s0 = 250nm is shown.
The general behavior of the linewidth frequency dependence is not affected by the
direction of the external magnetic ﬁeld. The convex curvature is related to the high
modulation ﬁeld used to increase the signal-to-noise ratio. Additional measurements
showed no isotropic two-magnon relaxation channel due to, e.g., grain-grain effects
[61] in these polycrystalline samples. When the external magnetic ﬁeld is applied
perpendicular to the stripes, the behavior of the linewidth-frequency dependence
becomes non-monotonous and is related to the two-magnon scattering process, which
is known to be activated in such a conﬁguration. One ﬁnds a large peak at 12.7GHz
and two smaller ones at 5.4 and 21.2GHz. These appear only for the direction
17.
Spin Dynamics in the Time and Frequency Domain 53
(a)
(b)
(c)
Fig. 5 Frequency dependence of the FMR linewidth of two samples structured with stripelike
defects. While the general behavior is the same within one single sample for B parallel to the stripes
(a) and B perpendicular to the stripes (b), for the latter conﬁguration additional peaks due to the
two-magnon scattering occur. Increasing the defects periodicity l from 250 to 400nm in the second
sample changes the position of the peaks and therefore the frequency dependence of the overall
spin relaxation. In (c) the frequency range is limited due to technical reasons. Solid lines are guides
for the eye
perpendicular to the stripes. Upon changing the periodicity to l = 400nm the spac-
ing of the relaxation rate (linewidth) peaks becomes smaller. This behavior is clearly
distinct from the original monotonous arcsin-like Eq.(14) frequency dependence. In
order to understand the appearance of these peaks one has to consider the disper-
sion relation of magnons parallel to the magnetization of a thin ﬁlm Eq.(3). In a
two-magnon process a uniform magnon with q||0 is scattered into a nonuniform state
with the same energy and different wave vector q||S , as shown in Fig.3. In order to
ﬁnd the wave vector of such a ﬁnal-state magnon one needs to solve the equation
ω(q|| = 0) = ω(q||S ). The wave vector of the ﬁnal-state magnons qS(ω) can be
calculated using the values of the effective perpendicular ﬁeld, anisotropy ﬁelds, and
18.
54 M. Farle et al.
g factor. The scattering process itself is enabled by the scattering ﬁeld, which couples
the uniform with the ﬁnal-state magnons. The coupling strength and consequently
the FMR linewidth scale with the square of the Fourier transform of the scattering
ﬁeld for q = qS. Using this model a very good qualitative agreement with the theory
has been achieved [28].
3.3 Spin-Torque Ferromagnetic Resonance
Spin-torque ferromagnetic resonance (ST-FMR) is an alternative approach to mea-
sure spin dynamics in magnetic nanostructures [62–72]. The general approach is
quite straightforward; an ac current is applied to a magnetic nanodevice that exhibits
either giant magnetoresistance or tunneling magnetoresistance, and a dc voltage is
generated that has a resonant structure when the ac frequency matches the resonance
condition for FMR. The physical mechanism that gives rise to the dc voltage may
be understood as follows. In a process commonly referred to as spin-momentum-
transfer, or spin-torque, the non-equilibrium spin currents generated in such a device
due to charge current ﬂow between the different magnetic layers necessarily impart
angular momentum to the magnetic layers in the device due to the sharp gradient in
the spin current at the surface of a magnetic conductor.1 The resultant ac torque at
the surface of the magnetic layer gives rise to motion of the magnetization, thereby
causing an ac variation in the device resistance. If the device resistance has a com-
ponent that is in-phase with the ac current, rectiﬁcation gives rise to a dc voltage. As
will be shown below, the rectiﬁcation is maximized when the excitation frequency
approaches the FMR frequency, though the details of the voltage signal near reso-
nance are strongly dependent on the symmetry of the spin torque in the structure.
Let U be the magnetic free energy for a rigid magnetic body. The equation of
motion for magnetization M in a ﬁeld H = − |γ | dU dmx ˆx + dU dmy ˆy is
given by
dM
dt
= − |γ | μ0 1 + α ˆm× M × H −
Js
δ
ε⊥ + ε|| ˆm× ˆm × ˆs (15)
where γ is the gyromagnetic ratio, μ0 is the permeability of free space, α is the
Landau-Lifshitz damping parameter, Js is the transverse spin-current-density inci-
dent upon the magnet, δ is the thickness of the magnetic layer, ε⊥ is the efﬁciency of
the perpendicular, or “ﬁeld-like” spin-torque, ε|| is the efﬁciency for the parallel, or
“damping-like” spin-torque, and ˆs is the polarization direction of the spin-current.2
The spin-current density has units of energy density, J/m3. For all-metal systems, it
1 For a more detailed description of spin torque, see Chap.2 by J. Lindner et al. in this book.
2 A similar equation is presented in Chap.2 by J. Lindner et al, though in terms of the Landau-
Lifshitz-Gilbert damping phenomenology rather than the Landau-Lifshitz formulation employed
here. In the limit of small damping, both equations are equivalent.
19.
Spin Dynamics in the Time and Frequency Domain 55
is generally understood that ε⊥ ε||. However, both data and theory indicate that
ε⊥ and ε|| are of comparable scale for magnetic tunnel junctions (MTJs), though
they have very different dependencies on the bias voltage applied across the tunnel
barrier [69].
For the case of ﬁeld-driven FMR (FD-FMR) with Js = 0, an ac ﬁeld hac =
h0e−iωt ˆy, and M ∼= mx ˆx + my ˆy + Ms ˆz, where mx , my Ms, the excitation
torque-density NF M R = μ0M × hac is
NF M R
∼= −μ0 Msh0eiωt
ˆx (16)
Thus, the excitation torque is necessarily at right angles to the excitation ﬁeld. To
understand the relationship of the magnetization to the excitation torque, we need to
consider the small-amplitude motion of the magnetization as a function of excitation
frequency, which can be easily derived from the Polder susceptibility tensor for the
Landau-Lifshitz equation of motion,
mx
my
= χ
hx
hy
(17)
where
χ ∼=
fM
f 2
0 − f 2 − i f f
fy + iαf −i f
i fx fx + iαf
(18)
with f = ω 2π, fM = |γ | μ0 Ms 2π, f 2
0 = fx fy, f = α fx + fy ,
fx,y = |γ | Ms d2U dm2
x,y , and U does not include the excitation ﬁeld.3 If
we consider the simplest high symmetry case with fx = fy = f0 and α fx,y f ,
the equation of motion for the component of magnetization parallel to the applied ac
ﬁeld becomes
my =
f0 fM h0
f 2
0 − f 2 − i2αf f0
(19)
In the limit of f f0, we have my = fM f0 h0; my is 180◦ out-of-phase with
the excitation torque NF M R along the x-axis, as depicted in Fig.6. At resonance with
f = f0, we have my = i 2α fM f0 h0; my is 90◦ advanced relative to NF M R
and 90◦ retarded relative to hac, but mx is now 180◦ out-of-phase with NF M R. The
resonance condition is shown schematically in Fig.6. This is an important general
result of ferromagnetic resonance that is independent of the excitation source: m · ˆx
and NF M R · ˆx are anti-phased on resonance such that the excitation torque acts purely
to counteract the damping torque, thereby maintaining a steady-state precessional
3 This particular form of the susceptibility tensor presumes that d2U dmx dmy = 0, i.e. the x
and y coordinates have been chosen to lie along principal axes of the anisotropy, and the applied
ﬁeld is perpendicular to the x − y plane.
20.
56 M. Farle et al.
(a) (b)
Fig. 6 Sketch of excitation torque acting on magnetization in ﬁeld-driven FMR
orbit of maximum amplitude.4 We will return to this point when we discuss the case
of spin-torque FMR below.
The output signal for a ﬁeld-driven FMR measurement depends on the type of
detection method. If the detection is based upon an inductive measurement, then we
have
V = i2πμ0 f Amy (20)
Now we will consider the case of spin-torque FMR (ST-FMR) with hac = 0.
The device structure now consists of two magnetic layers: A ﬁxed reference layer
that sets the direction of the spin current polarization, and an excited layer. Let us
again assume small-amplitude magnetization motion of the excited layer about the
saturation direction along ˆz. Let the polarization of the absorbed spin current ˆs lie in
the y-z plane, as depicted in Fig.7. When the ac spin current is Jac = J0e−iωt , the
excitation torque density NST is
NST
∼=
J0
δ
ε⊥ ˆx + ε|| ˆy eiωt
(21)
This allows us to deﬁne an effective ac excitation ﬁeld hST for the purposes of
calculating the magnetization response, where
hST =
|γ |J0eiωt
2π fM δ
ε|| ˆx − ε⊥ ˆy (22)
The relationship between the spin-current polarization vector ˆs and the effective
spin torque ac ﬁeld hST is shown in Fig.7. Let us now examine the signal produced
by the spin-torque excitation. The output signal V (t) due to giant magnetoresistance
4 One must remember that the magnetization and angular momentum are antiparallel for electrons.
Thus, a torque that is antiparallel to the magnetization will act to increase the magnetization along
the torque.
21.
Spin Dynamics in the Time and Frequency Domain 57
Fig. 7 Cartoon sketch of excitation torque acting on magnetization in spin-torque FMR
is given by
V (t) =
Re [I (t)] R
Ms
Re [m (t)] · ˆs
=
1
4
R
Ms
I (t) + I∗
(t) [my(t) + m∗
y(t)] sin(θ)
=
1
2
|γ |J0eiωt
2π fM δ
·
I0 R
Ms
cos(ωt)
fM (i f ε|| − fx ε⊥)
f 2
0 − f 2 − i f f
eiωt
+ cc sin(θ)
(23)
where θ is the angle between the magnetizations of the reference layer (the presump-
tive source reservoir for the spin current) and the excited layer. The resultant voltage
has a dc component Vdc given by
Vdc =
1
2
|γ |J0
2π FM δ
·
I0 R
Ms
fM (i f ε|| − fx ε⊥)
f 2
0 − f 2 − i f f
+
fM (i f ε|| − fx ε⊥)
f 2
0 − f 2 + i f f
sin(θ)
=
|γ |J0
2πδ
·
I0 R
Ms
ε⊥ fx ( f 2
0 − f 2) + ε|| f2 f
( f 2
0 − f 2) + ( f 2 f )2
sin(θ) (24)
We immediately see that the parallel spin torque gives rise to an even-symmetry
resonance response, whereas the perpendicular spin torque results in an odd-
symmetry resonance spectrum. We can understand this quite easily since we know
that the time-varying effective resistance is proportional to m · ˆy, and NST · ˆy is
180◦ out-of-phase with my when on resonance. Thus, only the y-component of the
spin torque contributes to the output signal when on resonance, resulting in a peak
amplitude that is proportional to ε||. Conversely, NST · ˆx due to the perpendicular
component of spin torque is 180◦ out-of-phase with mx when on resonance, but any
voltage signal due to NST · ˆx is necessarily 90◦ out-of-phase with the excitation spin
current, resulting in an odd-symmetry response curve.
An important prerequisite for the measurement of ST-FMR, as seen in the Eq.(24),
is the mis-orientation of the active and reference layers. To accomplish this, various
22.
58 M. Farle et al.
Fig. 8 Examples of the ﬁrst ST-FMR spectra obtained with a magnetic tunnel junction device. The
data show how the resonance frequency depends on an in-plane applied magnetic ﬁeld, as expected
for FMR. From Ref. [62]
approaches have been successfully used. For example, use of materials with greatly
differing magnetic moment for the active and reference layers can result in strong
misalignment of the magnetization orientation for the case of a perpendicular applied
ﬁeld.
While ST-FMR has yielded some of the ﬁrst data for FMR in individual nanoscale
magnetic structures, it suffers from inﬂexibility with regard to the thickness of the
structure in question. This is immediately apparent in Eq.(24), where we see that the
ST-FMR signal scales inversely with device thickness as a result of the interfacial
nature of the spin-torque effect. Thus, only very thin devices are amenable to such
measurements, leaving unanswered questions as to the role of phenomena such as
spin-pumping in determining the overall damping in nanomagnets.
Spin-torque FMR was ﬁrst demonstrated by Tulapurkar et al., by use of a
100 × 200nm MgO-based magnetic tunnel junction (MTJ) device with a TMR ratio
100% and a zero-bias, low-resistance of 150ohms [62]. The applied magnetic ﬁeld
was in the ﬁlm plane of the device. The device was excited at room temperature by
ac currents ranging from 200 to 640 μA. The output dc voltage scaled quadratically
with excitation current as expected for a rectiﬁcation effect, and output signals as
large as 35 μV were reported. Spectra were obtained by sweeping the excitation
frequency, an example of which is shown in Fig.8. The presented spectra exhibited a
single peak at the resonance frequency with both even and odd symmetries, indica-
tive of both the in-plane and perpendicular components of spin torque in the MTJ, as
theoretically predicted for such devices [12]. The resonance frequency scaled with
23.
Spin Dynamics in the Time and Frequency Domain 59
applied dc magnetic ﬁeld, and ﬁtting of the data with the Kittel equation yielded an
in-plane anisotropy of 176 Oe and an effective magnetization of 12.8 kOe. However,
a dc bias voltage was not applied to the device, thus precluding any determination
of the bias dependence for the different spin torque components in this particular
device.
The ﬁrst demonstration of ST-FMR in an all-metallic current-perpendicular-to-
plane giant-magnetoresistive (CPP-GMR) device was reported by Sankey et al., for
a 30×90nm device with a 20nm-thick Permalloy reference layer and a 5.5nm-thick
Py65Cu35 active layer [2]. The measurements were performed at cryogenic tempera-
tures (<10K), presumably to enhance the signal-to-noise ratio of the measurement.
The applied magnetic ﬁeld was out of the ﬁlm plane and of sufﬁcient strength to satu-
rate the active layer magnetization out of the plane, while insufﬁcient to do the same
for the reference layer. The excitation currents ranged from 12 to 990 μA, and the
maximum output signal was approximately 5 μV. Spectra were obtained by sweep-
ing the excitation frequency, and multiple peaks were reported, indicative of multiple
excitation modes in both the active and reference layers. In the absence of a dc bias
current, the resultant spectra exhibited even symmetry about the resonance frequency
at low ac currents. However, at high ac currents, the spectra acquired a distinct asym-
metry that suggests nonlinear magnetization dynamics [9]. For these measurements,
a dc current was also applied to modify the effective damping of the active layer,
as shown in Fig.9, which also includes an exemplary spectrum for zero dc current.
Analysis of the data for linewidth vs. dc current yielded a zero-current damping of
α = 0.04 and a critical current (α = 0) of Ic = 0.4 mA at an applied ﬁeld of 0.535T.
Conventional room-temperature FMR measurements of unpatterned blanket ﬁlms of
the same composition as the active layer yielded a = 0.021. It was conjectured by
the authors that the discrepancy in damping could be attributed to exchange coupling
between the patterned active layer and an antiferromagnet oxide on the edges of
the device that is below its blocking temperature for such cryogenic measurements.
The absence of such extreme damping enhancement in subsequent room temperature
measurements, as discussed below, corroborated this conjecture. However, an erro-
neous formulation for the dependence of the frequency-swept linewidth on damping
was used for the data analysis. This was addressed in a subsequent publication from
the same group, discussed below [66].
A theoretical treatment of ST-FMR in CPP-GMR devices was initially presented
by Kupferschmidt et al. [64]. Their approach was to ﬁnd a self-consistent solution of
the charge- and spin-current propagation through a one-dimensional structure sub-
ject to appropriate boundary conditions. The methodology included an accounting
for the reactive emission of spins from precessing ferromagnets into the nonmagnetic
spacers, also known as spin pumping [43]. An important ﬁnding from the theoretical
analysis was the contribution of the non-equilibrium spin accumulation in the non-
magnetic spacer layer to the dc voltage signal due to the generation of a nonzero dc
chemical potential at the various ferromagnet/conductor interfaces within the device.
It was determined that the contribution of the spin emission component to the net
dc voltage signal was comparable to that due to simple rectiﬁcation when the spin
pumping component of the damping was of the same scale as the intrinsic damping.
24.
60 M. Farle et al.
To date, however, an experimental conﬁrmation of this result remains lacking. A
subsequent theoretical analysis by Kovalev et al., using similar methods, arrived at
the same conclusion [65]. Another important result shared by both theories is the
manifestation of an odd-symmetry component of the resonance even if ε⊥ = 0.
The origin of the odd-symmetry is purely geometrical in origin, stemming from the
possible misalignment of the effective spin-torque ac ﬁeld hST with respect to the
principle anisotropy axes of the device [64].
Fuchs, et al. ﬁrst reported room temperature measurements for 50 × 10 nm all-
metal CPP-GMR nanopillars [66]. An in-plane applied magnetic ﬁeld was used. As
was presented in the ﬁrst work by the same group [63], the damping was inferred by
measuring frequency-swept linewidth as a function of dc current, then using a linear
ﬁt to determine the zero-current linewidth. Since the dependence of frequency-swept
linewidth on damping is proportional to the sum of the stiffness frequencies fx and
fy, it is necessary to determine the effective anisotropy that establishes the FMR
frequency. To see this, we consider the dependence of frequency-swept linewidth on
damping,
f = α( fx + fy) (25)
where fx and fy are deﬁned earlier in this chapter. Let us now consider the derivative
of resonance frequency with respect to applied ﬁeld,
d f0
d H
=
γ μ0
4π f
( fx + fy) (26)
Thus,
α =
γ μ0
4π f0
f
d f0
d H
(27)
We clearly see that determination of the damping from frequency-swept data
is facilitated by a commensurate determination of the resonance frequency depen-
dence on applied ﬁeld. However, such data were not forthcoming in Ref. [66] which
required an estimation of the stiffness frequencies by modeling the active elements
as uniformly magnetized elliptical cylinders. The systematic errors associated with
such an estimate were not determined. Nevertheless, the authors concluded that the
extracted values for the zero-current damping were essentially identical (with 50%
error bars) to the measured values for unpatterned blanket ﬁlms presented elsewhere
in the literature.
A more accurate determination of damping in nanostructured CPP-GMR devices
was presented by Chen et al. [67, 68]. This work used a Co/Ni multilayer active layer
with perpendicular anisotropy, although the interfacial anisotropy was insufﬁcient
to overcome the intrinsic shape anisotropy for a thin ﬁlm. The applied magnetic
ﬁeld was perpendicular to the ﬁlm plane. The large difference in the net anisotropy
25.
Spin Dynamics in the Time and Frequency Domain 61
(a) (b)
Fig. 9 Example of ST-FMR spectrum and dependence of spectral linewidth on dc current for
metallic GMR device. a An example of a ST-FMR spectrum without any additional dc current.
The applied ﬁeld of slightly more than 0.5T is oriented out of the ﬁlm plane and is sufﬁcient
to saturate the excited layer out of the ﬁlm plane. b The dependence of the ST-FMR linewidth
on dc current. The observed linear dependence is in agreement with theoretical predictions (see
Eq. 15). The critical current Ic for self-oscillations is extrapolated from a linear ﬁt to the data. From
Ref. [63]
of the active and reference layers allowed for the requisite misalignment of the
magnetization angles over a wide range of applied magnetic ﬁeld. Here, the ﬁeld-
swept linewidth was determined as a function of excitation frequency, permitting
an unambiguous determination of the damping parameter as α = 0.033 ± 0.003,
which was within error bars of a conventional FMR measurement for an unpatterned
multilayer ﬁlm with α = 0.036 ± 0.002. The linewidth vs. frequency data for both
ST-FMR and FD-FMR are presented in Fig.10. Similar to Fuchs et al., the authors
concluded that patterning of the active layer nanomagnet did not cause a detectable
change in the intrinsic damping. While micromagnetic simulations predict [73] and
data have shown [74, 75] that multiple modes should be present in such ﬁnite-sized
active layers, the experimental signal-to-noise was not sufﬁcient to clearly determine
the presence of such higher order modes. In addition, the shift of the device resonance
frequency from that of the unpatterned ﬁlm was approximately a factor of two less
than what simulations predicted for the lowest order normal mode. The discrepancy
between modeling and experiment was not explained, though it was conjectured
that the actual device size may have been substantially different from the nominal
dimensions of 50 × 150 nm.
The use of ST-FMR to study tunnel junction devices was revisited by Sankey et al.
in an IBM/Cornell collaboration [69]. The devices under study (500 × 100 nm and
50 × 150 nm) utilized a CoFeB (3nm)/MgO (1.25nm)/CoFeB (2.5nm) stack. In this
case, the authors were less concerned with the damping of the active layer. Instead,
the intention was to determine the dependence of the spin torque on bias voltage.
It was observed that the ST-FMR lineshape exhibited both even and odd symmetry
26.
62 M. Farle et al.
(a) (b)
Fig. 10 Dependence of ST-FMR spectral peak position (a) and linewidth (b) on microwave fre-
quency. The applied ﬁeld is perpendicular to the plane of the device. The linewidth for FD-FMR is
also shown in (b) with the ﬁlled square data points. The linewidth exhibits classic linear dependence
on frequency, as expected for Landau-Lifshitz damping processes. From Ref. [67]
components Eq.(24) that had different dependencies on bias voltage. It was found
that the parallel, or “damping-like”, torque (referred to as the “in-plane” torque in
Ref. [69]) only displayed a weak dependence on bias voltage for voltages as large as
0.4V, even though the TMR ratio was reduced by a factor of two at such a bias voltage.
In addition, the perpendicular, or “ﬁeld-like”, torque was comparable in magnitude
to the parallel torque over the range of bias voltages, although its dependence on bias
voltage appeared linear with a zero-intercept at zero bias.
Nonlinear resonance effects were indicated by Chen, et al. in another work from
the NYU group that utilized CPP-GMR structures with Co/Ni active layers [70]. It
was found that the ﬁeld-swept resonance lineshape took on a distinctive “saw-tooth”
shape with increasing microwave current excitation, as shown in Fig.11. Such a line-
shape results in a shift of the peak resonance frequency to lower applied magnetic
ﬁelds with increasing microwave excitation. The saw-tooth shape is a tell-tale sig-
nature of nonlinear bistability in FMR measurements [76–78]. However, hysteresis
of the lineshape, another essential feature of bistability, was very weak in compar-
ison to macrospin simulation results. The authors speculate that thermally driven
ﬂuctuations might obscure the observation of such hysteretic effects.
ST-FMR has also been demonstrated with point-contact spin-torque devices,
where the active layer is not lithographically patterned [71]. Instead, the current is
injected into a blanket spin-valve stack using a lithographically deﬁned point contact
[79]. Again, the extracted value of damping was found to be in rough agreement with
previously published results for the same material as the active layer, a Co/Ni multi-
layer with a net perpendicular anisotropy of only 64 mT. In addition, the determined
ST-FMR resonance frequency dependence on applied ﬁeld at zero bias current was
found to coincide with the onset frequency of auto-oscillations at the critical current,
demonstrating that the excitation generated by dc current in this particular device
was of small amplitude at threshold.
27.
Spin Dynamics in the Time and Frequency Domain 63
Fig. 11 ST-FMR spectra ver-
sus ac current amplitude for
metallic GMR device. From
bottom to top, the rf current
amplitude was 1.4, 2.1, 3.3,
4.6, 6.2, 7.8, and 9.0mA. The
saw-tooth shape for large exci-
tation amplitudes is evidence
for large amplitude precession
of the active layer magneti-
zation. The shift in the peak
resonance frequency from that
for small excitation amplitude
is linearly proportional to the
decrease in the z-component
of the magnetization at the
maximum precession ampli-
tude. From Ref. [70]
4 Ferromagnetic Resonance Detection in the Time Domain
4.1 Time Resolved Kerr Microscopy
Time resolved Kerr microscopy is a very convenient technique to study the mag-
netization dynamics in the time domain. In this method light from a pulsed laser is
coupled into an optical microscope with polarization analysis. Due to the magneto-
optic Kerr effect (MOKE) the polarization of light that is reﬂected from a magnetic
sample is altered as a function of the orientation of the magnetization vector. Here
this effect is used to study the dynamics of the magnetization vector in the sample.
Time Resolved (TR)-MOKE is a pump-probe technique where the sample is peri-
odically excited by an external stimulus (e.g. optical pulse or magnetic ﬁeld pulse)
which is synchronized to the laser pulses. The time resolution of such experiments
is only limited by the duration of pump and probe events. For the experiments dis-
cussed in the following a Ti:sapphire laser is used to generate light pulses of 150fs
duration at a repetition rate of 80MHz and at a central wavelength 800nm. The laser
light is split into two parts, which are referred to as pump and probe beams. The
pump pulses are used to trigger magnetic ﬁeld pulses which excite magnetization
dynamics in the sample. The probe pulses sample the state of the system at a delay
time t which is determined by the time delay between pump and probe pulse. In the
present experimental setup the detection of the magneto optic Kerr effect is such that
only the polar component of the magnetization vector contributes to the measured
signal. However in principle it is possible to detect all components of magnetization
vector in TR-MOKE experiments using a more sophisticated detection scheme [80].
In order to measure the time dependence of the magnetization an opto-mechanical
28.
64 M. Farle et al.
delay stage can be used to scan the optical path of the pump pulses with respect to
probe events.
It is necessary to perform TR-MOKE measurements in a stroboscopic fashion
since the signal of a single pump-probe event is too small to be detected. In order to
obtain a sufﬁcient signal to noise ratio the same experiment is typically repeated many
million times at a ﬁxed delay time while the pumping is modulated at a frequency
of a few kHz. This modulation allows lock-in detection of the small dynamic Kerr
signal. In addition, for experiments with pulsed excitation two conditions should
be fulﬁlled. First, the relaxation of the system back into its ground state should be
completed before the next pump pulse arrives. For the experiments discussed here
the repetition rate of the laser is 80MHz, i.e. this relaxation should take place within
12.5ns. Second, the response of the system to the pump event has to be reproducible.
All stochastic processes, such as variations of the response due to slightly different
experimental conditions or thermal magnon excitation average out.
In the experimental setup the fundamental near infrared beam of the Ti:Sapphire
laser (λ ∼ 800nm) is focused into a lithium-borate (LBO) crystal, where the
light is partly frequency doubled to λ ∼ 400nm by second harmonic generation.
The spatial resolution xmin is obtained by scanning the sample laterally under the
objective lens of a microscope using a piezo-mechanical stage. The resolution is
diffraction-limited and determined by the numerical aperture of the objective lens
and the wavelength of the light. The objective lens that is used has a numeri-
cal aperture of NA = 0.90. Therefore a spatial resolution of xmin = λ
2NA ≈
230nm can be achieved. The the polarization state of the reﬂected light is ana-
lyzed by means of a Wollaston polarizer and the difference signal is measured
by two photo diodes. This difference signal is fed into a lock-in ampliﬁer and
sensitive to the time dependent magnetization state of the sample. In addition
the intensity i.e. the sum signal of both photo diodes represents the reﬂectivity of the
sample at the laser spot position. This signal allows to record the topography of the
sample simultaneously with the magneto-optic response.
In the following sections experiments with pulsed and continuous wave (cw)
excitation are discussed with the aim to illustrate the potential of the TR-MOKE
technique.
4.2 Pulsed Experiments
In this section two experiments with pulsed excitation will be discussed. In the ﬁrst
experiment short current pulses are generated by optical pump pulses in a photo-
conductive switch. In a second experiment microwave bursts are generated by a
signal generator. These rf-currents are coupled into a micro structured transmission
line and the corresponding rf-magnetic ﬁeld excites magnetization dynamics in the
magnetic sample. The pump-probe experiments allow to record the ring down of the
excitation by measuring the Kerr signal as a function of the delay time between pump
and probe pulses. In the ﬁrst experiment the interaction between a magnetic vortex
29.
Spin Dynamics in the Time and Frequency Domain 65
Fig. 12 Illustration of the time resolved Kerr microscopy setup. Part of the fundamental infrared
beam of the Ti-Sapphire laser (∼800nm) is frequency doubled using a LBO crystal. This frequency
doubled blue beam (∼400nm) probes the perpendicular magnetization component by means of
the polar magneto-optic Kerr effect. The red laser pulses are delayed by means of a mechanical
delay stage and focused onto a fast photo diode which triggers the generation of phase-synchronized
microwaves. The microwave current passes through the coplanar waveguide structure of the sample,
leading to an rf-magnetic ﬁeld h which excites the precession of the magnetization. The sample is
placed on a piezo scanning stage which is used to scan the sample laterally under the ﬁxed laser
focus. Static magnetic ﬁelds H can be applied in any direction in the sample plane by a rotatable
electromagnet
core and spin wave eigenmodes in a magnetic disk will be examined. In the second
experiment the propagation of spin-wave pulses which are excited by microwave
bursts is studied.
4.2.1 Interaction Between Spin-Waves and a Vortex Core
In this experiment the magnetization in a disk of Ni80Fe20 with a diameter of 1.5 μm
and a thickness of 15nm is excited by in-plane magnetic ﬁeld pulses. The current
pulses which create an in-plane magnetic rf pumping ﬁeld are generated by pulsed
30.
66 M. Farle et al.
(a)
(d)
(b)
(c)
Fig. 13 Principle of imaging of eigenmodes by local Fourier transformations. a ﬁrst a series of
images of the Kerr contrast is recorded by TR-MOKE at various delay times after pulsed excitation
of a Ni80Fe20 disk with a diameter of 1.5 μm and a thickness of 15nm. Second the time dependence
in each pixel of these images (shown in b) is Fourier transformed (c). d shows the amplitude and
phase of the Fourier transformation (FFT) visualized as a function of frequency. Adapted from [82]
illumination of a photo-conductive switch as illustrated in Fig.12 and the magnetic
disk is placed on top of the signal line of a coplanar waveguide. The magnetization
dynamics is recorded by TR-MOKE. For a given time delay between pump and probe
pulses snapshots of the magnetic excitation as shown in Fig.13a can be recorded. For
each pixel of the snapshot the time evolution of the magnetic excitation can be plotted
as can be seen in Fig.13b. The application of a Fourier transformation to these time
dependent data allows to identify the spin-wave eigenmodes [81]. In the frequency
domain one can identify peaks corresponding to the excited eigenmodes (Fig.13c).
The amplitude and phase of the Fourier transformed spectra can be reassembled to
form images as a function of frequency (see Fig.13d). The eigenmodes are clearly
visible. An in-plane ﬁeld pulse applied to vortex state with its circulating magneti-
zation mostly excites the ﬁrst azimuthal mode (1, ±1) as the M × hrf term has the
opposite sign on both sides of the disk [82]. In addition also the magnetic vortex core
is excited to gyrate around the center of the disk.
From the Fourier transformed data that were spatially averaged over one half of the
disk as shown in Fig.14a one can see that the intrinsic degeneracy of the clockwise
and counter clockwise rotating ﬁrst azimuthal modes (1, +1) and (1, −1) is lifted. In
the amplitude and phase images at both peaks one can see that they correspond to the
ﬁrst azimuthal mode. However the phase of the lower peak rotates clockwise while
the phase of the higher frequency peak rotates counterclockwise. This splitting is a
31.
Spin Dynamics in the Time and Frequency Domain 67
(a) (b)
Fig. 14 a Fourier spectrum of measured dynamics averaged over one half of a Ni80Fe20 disk with
a diameter of 1.5 μm and a thickness of 15nm. b Spectral amplitude and phase images of the two
azimuthal modes (1, +1) and (1, −1) measured by TR-MOKE. Adapted from [82]
consequence of the interaction of the spin-wave eigenmodes with the vortex core. We
have demonstrated in [82] that the removal of the magnetic vortex core (by etching
a hole in the center of the disk) results in a disappearance of the splitting. Guslienko
et al. have shown theoretically that the dynamic interaction between the rotating
spin-waves and the vortex core motion is responsible for the mode splitting [83].
4.2.2 Spin-wave Propagation
In order to study the propagation of spin-waves extended magnetic structures are
needed. For this purpose this section discusses the propagation of spin-wave packets
in large Ni80Fe20 ﬁlm structures upon pulsed microwave excitation. Traditionally the
spin-wave propagation and the propagation of non-linear spin-wave packets (bullets
or spin-wave solitons) has been investigated mostly for the ferrimagnetic insulator
Yttrium Iron Garnet due to its small intrinsic damping. In experiments employing
inductive detection the propagation of spin-waves in ferromagnetic thin Ni80Fe20
ﬁlms was observed over distances of up to 50 μm [84]. Here the direct TR-MOKE
observation of the propagation of spin-waves in a 20nm thick continuous Ni80Fe20
ﬁlm is demonstrated.
The sample considered in the following consists of a 20nm thick Ni80Fe20 ﬁlm
with lateral dimensions of 200 × 200 μm2 patterned onto a GaAs substrate. Subse-
quently a coplanar stripline (CPS) is patterned over one edge of the Ni80Fe20 ﬁlm
using optical lithography (see Fig.15a). A microwave generator is synchronized to
the 80MHz repetition rate of the Ti:Sapphire laser system in order to provide a
phase-stable correlation between microwave excitation and the laser probe pulses. In
addition a frequency mixer is added into the microwave circuit in order to generate
32.
68 M. Farle et al.
(a) (b)
Fig. 15 a Sample layout. The 200nm thick CPS fabricated from Au is placed over one edge of the
Ni80Fe20 ﬁlm. b Propagation of spin wave packets. Proﬁle of the 4GHz microwave pulse with a
duration of 1ns (lowest line) and scans in time of the spin wave packet at various distances from the
CPS (the distance in microns is indicated above the individual lines). The curves have been offset
for clarity. Adapted from [85]
microwave ﬁeld pulses as short as 1ns at a carrier frequency given by a multiple of
the 80MHz repetition rate of the laser. By measuring the Kerr signal as a function
of delay time at various distances from the excitation source (waveguide) one can
follow the propagation of a spin-wave packet directly. This allows one to observe the
propagation of spin-wave packets in space and time as shown in Fig.15b.
For a continously applied microwave excitation the response of the magnetization
is given by the product of the q-dependent excitation and the q-dependent susceptibil-
ity. The q-vector where this product has a maximum is determined by the waveguide
and the direction and magnitude of the applied magnetic ﬁeld. This means that the
magnetic ﬁlm ‘picks’ the wave vector with the largest susceptibility from the Fourier
spectrum of the CPS at a given driving frequency. By measuring line scans as a
function of time the phase velocity vPh of the spin-waves can be directly determined
from the slope x/ t of the oscillatory signal. The phase velocity can easily be con-
verted into a q-vector: q = 2π f
vPh
. By performing such measurements as a function of
frequency one can experimentally determine the dispersion relation for spin-waves
[85].
When only short bursts of microwave excitation are applied to the sample one can
study the propagation and dispersion of spin-wave pulses. Delay scans recorded at
various distances from the CPS are shown in Fig.15b. It can clearly be observed how
the microwave burst triggers a spin-wave packet that propagates along the x-direction
and broadens considerably as a function of time due to dispersion. In addition, the
signal is damped according to the intrinsic damping parameter of the Ni80Fe20 ﬁlm.
Nevertheless, we are able to detect a response at distances up to 80 µm from the CPS.
From these data of the pulsed excitation the group velocities of the spin-wave packets
are readily determined. The measured group velocities vG = ∂ω
∂q are highest (up to
17km/s) when the wave vector of the spin-wave and magnetic ﬁeld are orthogonal
(Damon Eshbach geometry), while they are smaller for intermediate ﬁeld directions
33.
Spin Dynamics in the Time and Frequency Domain 69
806040200
-1
0
1
microwave
modulation[a.u.]
probepulse
ampl.[a.u.]rf-field[a.u.]
time [ns]
12.5 ns
Fig. 16 Synchronization between continuous microwave excitation and laser probe pulses. Due to
the repetition rate of the laser, the magnetization is probed every 12.5ns. The microwave phase is
the same for each probe event. 180◦ phase modulation of the microwaves is performed with a low
frequency in the kHz-range. Note that at t = 40ns, the phase of the excitation ﬁeld is switched by
180◦
and close to zero when q-vector and applied magnetic ﬁeld are parallel (backward
volume geometry).
4.3 CW Experiments: Ferromagnetic Resonance
Instead of applying a short magnetic ﬁeld pulse or a microwave burst to the magnetic
system the sample can be excited by means of a cw rf-ﬁeld which is phase-locked to
the laser pulses [86]. By measuring the TR-MOKE signal as a function of the time
delay between microwave signal and optical probe one obtains the amplitude of the
oscillating out-of-plane component of the precession. In addition, the phase of the
response can be measured by comparing the phase of the Kerr signal to the phase of
the microwave signal measured by a sampling oscilloscope.
For a ﬁxed microwave frequency one can also measure ferromagnetic resonance
(FMR) spectra by sweeping the external ﬁeld. Depending on the relative phase
between the probe pulses and microwave ﬁeld, such FMR-TR-MOKE spectra are a
combination or real and imaginary parts of the rf-susceptibility. The expected line
shapes for real (in-phase) part χ and imaginary (out-of-phase) part χ of the sus-
ceptibility are shown in Fig.17. The static magnetization is assumed to point along
the x-direction and the tip of the precessing magnetization is assumed to precess
on a circular path in the y-z-plane due to the microwave excitation. The dots label
the position of the tip of M at the point in time when the probe pulse samples the
34.
70 M. Farle et al.
H0
m z
HR
H0
mz
HR
zz
[a.u.]
mz
[a.u.]
magneticfield[a.u.]
HR
zz
[a.u.]
mz
[a.u.]
magneticfield[a.u.]
HR
(a)
(b)
Fig. 17 Illustration of the different line shapes in Kerr-FMR measurements. (Left side)
z-components of the magnetization mz versus external magnetic ﬁeld H for two different microwave
phases. The static magnetization lies along the x-direction. The circles represent the precessing mag-
netization in the y-z-plane. The dots label the position of the tip of the magnetization vector for
different ﬁeld values at the moment when the probe pulses sample the polar component (mz).
(Right side) Depending on the phase correlation, the resulting spectra can have a symmetric (a) or
an asymmetric line shape (b)
z-component of M. Far away from resonance (H HR and H HR), the preces-
sion amplitudes are small, expressed by the smaller circles. At resonance (H = HR),
the precession amplitude is maximum. In addition, the phase between excitation ﬁeld
hrf and the precessing magnetization M has to be considered. For high magnetic
ﬁelds, hrf and M move in phase (ϕ = 0), since the frequency of the microwave ﬁeld
excitation is much lower than the resonance frequency. The phase changes gradu-
ally from 0 to π/2 when the external ﬁeld is decreased. At resonance, the phase
lag of the precessing magnetization behind the excitation ﬁeld is exactly π/2. In
order to perform such measurements a microwave generator is synchronized with
the laser pulses and an electronic line stretcher allows precise adjustment of the
microwave phase. The rf-signal is delivered to the sample by a coplanar waveguide.
In order to ensure both the excitation of the sample and the phase synchronization
of the microwave signal with the probe laser pulses the microwave signal is mon-
itored using a sampling oscilloscope. The synchronization between excitation and
probe pulses is shown schematically in Fig.16. Since the microwave phase is mod-
ulated by 180◦ (cf. Fig.16), the output signal from the lock-in ampliﬁer represents
the difference signal of magnetization vector from opposite sides of the precession
cone (cf. Fig.17). TR-MOKE with cw excitation allows to combine two experimen-
tal techniques: ferromagnetic resonance (FMR) and time-resolved scanning Kerr
microscopy. FMR-TR-MOKE allows one to perform spatially resolved resonance
measurements. Thus this technique can be used to image magnetic modes in con-
ﬁned magnetic structures or to visualize local variations of the internal ﬁelds [87].
35.
Spin Dynamics in the Time and Frequency Domain 71
In the following the capabilities of this technique will be demonstrated by two
examples. First this technique is used to measure the dynamics due to pure spin
currents in metallic multilayers. In the second example local magnetic resonance
spectroscopy is used to obtain the magnetic anisotropies in stained nano-structures
of a magnetic semiconductor.
4.3.1 Spin Pumping in Magnetic Bilayers
In this section the FMR-TR-MOKE technique is used to study the magnetization
dynamics due to pure spin currents. Spin polarized currents offer the possibility to
exert a large torque on nano-magnets [88, 89]. In recent years current induced mag-
netization dynamics was successfully demonstrated in magnetic nanostructures [79,
90, 91]. Such current induced dynamics is mostly studied in spin valve structures
using columnar nano-magnets. In a nonlocal crossed wire geometry even the switch-
ing of a magnetic nano-particle by a spin current was demonstrated [92]. In all these
experiments the spin polarized currents are driven by charge currents. The precession
of the magnetization in a ferromagnet which is in contact with a normal metal layer
leads to the emission of a pure spin current into the normal metal [93]. This effect
is known as spin pumping and leads to an increased damping for the magnetization
dynamics in the layer that emits the spin current [94, 95].
In the FMR-TR-MOKE experiment that is discussed in the following it is shown
that rf-precession can be excited by the absorption of a pure spin current which is
generated by spin pumping. For this an epitaxial stack of layers consisting of Fe
and Au grown on GaAs(001) is investigated. It is known that the magnetic layers
in Au/Fe/Au/Fe/GaAs structures are dynamically coupled via spin pump and spin
sink effects [17, 95]. In such a magnetic bilayer the magnetization dynamics in the
presence of spin pump and spin sink effects can be described by the following coupled
set of modiﬁed Landau-Lifshitz-Gilbert equations [95]:
dmi
dt = −γμ0 [mi × Heff] + αi mi × dmi
dt + αi
SP mi × dmi
dt − mj ×
dmj
dt
(28)
where m1,2 are unit vectors along the instantaneous magnetization directions of the
two ferromagnetic layers F1 and F2. The strength of the spin pump and spin sink
effects is given by the parameter αSP = gμB
g↑↓
Ms
1
t1
, where t1 is the thickness of F1,
g↑↓ (in units of e2/h) is the real part of the spin mixing conductance [95] and μB is
the Bohr magneton. The exchange of spin currents is a symmetric concept and the
equation of motion for layer F2 can be obtained by interchanging the indices i j in
Eq.(28). The net spin current generated by layer F1 propagates away from the F1/N
interface [93] and is absorbed at the N/F2 interface if N is thinner or comparable to
the spin diffusion length (spin-sink effect) [96]. Conservation of angular momentum
requires that layer F1 looses spin momentum which leads to an increase of the Gilbert
damping parameter of layer F1. Subsequently, the spin current absorbed at the N/F2
36.
72 M. Farle et al.
(a) (b)
Fig. 18 a Calculated resonance frequency vs. applied ﬁeld for 20Au/10Fe/250Au/16Fe/GaAs(001)
(numbers are in monolayers) with the magnetic ﬁeld applied along the [110] direction of Fe.
The FMR frequencies for the 10Fe(F2) and 16Fe(F1) layers are shown in the red and blue lines,
respectively. Note, that the blue line is shifted upwards compared to the red line. This shift is caused
by the in-plane uniaxial interface anisotropy at the Fe/GaAs interface with the easy axis along the
[110] direction. Layer F2 has a weak cubic anisotropy with easy 100 directions. Above 20mT
both layers are aligned parallel with their resonance frequencies separated by several GHz. The
inset shows the experimental conﬁguration. b Optical image of the actual sample. The signal line
has a width of 30 μm. The magniﬁcation shows the Kerr signal of the 25 × 8 μm2 rectangle in a
bias ﬁeld of 65mT at a frequency of 8.08GHz. From [17]
interface creates an rf-torque on the magnetic moment in F2. Since F2 is an ultrathin
ferromagnet the interface torque results in a homogeneous precession of the layer F2
at the resonance frequency of F1. In an inductive FMR experiment this effect cannot
be observed directly since the rf-response is dominated by the FMR signal from F1.
The single crystalline magnetic double layer structures that are used in the exper-
iment are grown by molecular beam epitaxy in ultra high vacuum on GaAs(001)
substrates, further details can be found in [94]. The different interface anisotropies
of the two ferromagnetic layers can be used to split the resonance frequencies of
F1 and F2 by several GHz. The expected resonance frequencies for F1 and F2 as
a function of bias ﬁeld applied along the [110] direction are shown in Fig.18a. As
shown in Fig.18, for ﬁelds above 40mT the magnetic moments of layers F1 and F2
and the dc ﬁeld are collinear and parallel to the [110] direction of Fe.
A cw-signal of 10GHz was applied to the micro structured coplanar transmission
line (shown in Fig. 18b) and as expected from Fig.18a the FMR-TR-MOKE signal
for the layer F2 occurs at a ﬁeld of 96mT, as can be seen in Fig.19a. At the resonance
ﬁeld of layer F1 a typical antisymmetric line (corresponding to the real part of the
rf-susceptibility χ ) and a symmetric line (corresponding to the imaginary part of the
rf-susceptibility χ ) are found in the tails of the out-phase and in-phase rf-response,
respectively. These signals at the F1 resonance ﬁeld are in agreement with the spin
pumping theory. F2 is driven by the spin current generated by F1, see Eq.(28),
which is proportional to the time derivative of the rf-magnetization of layer F1.
37.
Spin Dynamics in the Time and Frequency Domain 73
(a) (b)
Fig. 19 a Measured real (red line) and imaginary (black line) parts of the perpendic-
ular rf-susceptibility of layer F2. A frequency of 10GHz was used and the magnetic
dc-ﬁeld was swept parallel to the [110] direction of Fe. The corresponding calculations
using Eq.(28) are shown as dotted lines. The inset magniﬁes the region of interest. b
The ratio of the signal amplitudes (FMR signal/ spin pumping signal) is plotted for a
series of samples with Au spacer layer thicknesses between 30 and 60nm. These data
allow one to estimate of the spin diffusion length for Gold to be λsd = 34nm. [97]
Therefore this driving is phase shifted by about π/2 with respect to the applied
rf-ﬁeld. Consequently, the additional driving due to spin pumping exchanges the
resonance line shapes for the real and imaginary parts in the rf-susceptibility. I.e. in
the imaginary (real) part of the F2 susceptibility has a contribution at the F1 resonance
which has the line shape of the real (imaginary) part of the susceptibility of F1, see
Fig.19a. All these experimental features are well reproduced by the spin pumping
theory using Eq.(28). The measured signal agrees with the calculations in its shape,
however due to spin relaxation in the Gold spacer layer the amplitude is reduced by
70 % compared to ballistic spin transport, (c.f. dashed lines in Fig.19a).
In the measurements the direct Kerr signal from the bottom layer is suppressed
using an optical compensator [17]. In addition one should point out that dipolar cou-
pling between the ferromagnetic layers e.g. caused by roughness would always lead
to a symmetric line at the F1 resonance but cannot result in the observed antisym-
metric line shape. Therefore one can ﬁrmly conclude that the signal measured at the
F1 resonance in Fig.19a is a sole consequence of the absorbed spin current in F2.
It is worthwhile to point out that the technique presented here can be used to
estimate the spin diffusion length in the metallic spacer layer [17, 97]. For this the
decay of the signal due to spin pumping is measured as a function of spacer thickness
andcomparedtotheory.ThisisshowninFig.19b.Fortheinterpretationitisimportant
to take spin diffusion effects into account [97]. The value one obtains for the spin
diffusion length from these data at room temperature in Gold is λsd = 34nm [97].
38.
74 M. Farle et al.
4.3.2 Local Magnetic Anisotropies
In this section it is shown that the FMR-TRMOKE technique can be used to deter-
mine the magnetic anisotropies with high spatial resolution. For this purpose mea-
surements of the magnetic anisotropy of are performed in a spatially resolved manner
on nanostructures of the magnetic semiconductor (Ga, Mn)As.
Due to the low Curie temperature of the diluted magnetic semiconductor, the
experiments are carried out low temperature in a microscope cryostat. The magnetic
properties of the diluted magnetic semiconductor (Ga, Mn)As have been studied
previously using ferromagnetic resonance, SQUID, magnetotransport or Hall-effect
measurements. In (Ga, Mn)As the magnetic anisotropies depend on temperature
and hole concentration [98]. It was shown that the magnetic anisotropies can be
manipulated by applying mechanical stress to the sample [99]. It has also been
demonstrated that the easy axis of the magnetization can be rotated by varying the
hole concentration using a strong electric ﬁeld [100]. However, these techniques do
not resolve magnetic anisotropies in (Ga, Mn)As micro-and nanostructures locally.
The experiments presented in the following show spatially resolved measurements
of the magnetic anisotropy with a resolution of 500nm. A (Ga, Mn)As ﬁlm grown
on GaAs(001) was investigated. Due to the lattice mismatch between (Ga, Mn)As
and GaAs this sample is compressively strained. The strain gives rise to a strong
perpendicular magnetic anisotropy with a hard axis along the ﬁlm normal. By pat-
terning a (Ga, Mn)As ﬁlm into small structures this strain can be partially relieved,
strongly affecting the magnetic anisotropies. The FMR-TR-MOKE approach com-
binestheadvantagesoftwoexperimentaltechniques:angle-dependentFMRprovides
direct access to the energy landscape and the magnetic anisotropies and TRMOKE
microscopy allows spatially resolved measurements. Thus these experiments can
serve to visualize local variations of the magnetic anisotropy.
In the following a 50nm thick Ga1−xMnxAs ﬁlm with a nominal Mn content x =
0.06 grown on a GaAs(001) substrate is studied. This sample has a Curie temperature
of 170K. Further details concerning the sample preparation can be found in [101].
The magnetic elements are deﬁned by electron beam lithography and dry etching
steps. The etch depth into the GaAs substrate is approximately 30nm. Stripes having
a width ranging from 200 nm up to 4 μm patterned along different crystallographic
directions ([100], [110], [010]) and disks with different diameters were prepared. For
the excitation of the magnetization with microwaves in the GHz-range a coplanar
waveguide was deﬁned in a subsequent lithography step. The magnetic elements are
placed in the gap between the 30 μm wide signal line and the ground plane resulting
in a out-of-plane rf-excitation, cf. Fig.20a.
In order to determine the magnetic anisotropies FMR spectra are recorded for a
series of applied ﬁeld angles. Fig.20b shows angle dependent FMR spectra for a
large 60 × 60 μm2 (Ga, Mn)As reference sample which represents the response of
on an isotropically strained ’unpatterned’ ﬁlm. The individual TR-MOKE spectra
are ﬁtted to Lorentzian line shapes in order to determine the resonance ﬁelds. The
resultingangulardependenceoftheresonanceﬁeldsisshowninFig.20.Byﬁttingthis
angular dependence the magnetic anisotropy constants in the free energy density can
39.
Spin Dynamics in the Time and Frequency Domain 75
(a) (b)
Fig. 20 a Sketch illustrating the waveguide and the rf excitation of the magnetic elements. b FMR
spectra for various angles ϕH of the magnetic ﬁeld in the ﬁlm plane (001) for f = 3.84GHz and
T = 7K for the reference structure. The resonance ﬁelds are obtained by ﬁtting the experimental
data to an asymmetric Lorentz function and are indicated by open dots. The red solid line represents
the ﬁt which is used to extract the anisotropy constants. From [101]
be determined [25, 101] : F = −μ0 M H (cos(ϕM − ϕH )) − 1
8 K4 (3 + cos 4ϕM) −
K2 sin2 ϕM − π
4 , where M is the magnetization and ϕM and ϕH are the angles
of the magnetization and the external magnetic ﬁeld H with respect to the [100]-
direction. K2 and K4 are the uniaxial and cubic in-plane anisotropy constants.
The angular dependence shown in Fig.20b (isotopically strained ﬁlm) is domi-
nated by the intrinsic cubic anisotropy K4. The difference in resonance ﬁeld observed
along the [110] and [1¯10]-directions is due to the in-plane uniaxial anisotropy K2 .
The experimental data can be ﬁtted well using the above energy density. The result-
ing anisotropy constants are K4 = 2.2 × 102 J
m3 , K2 = −1.1 × 102 J
m3 and
K2⊥ = −3.0 × 103 J
m3 .
Next, the patterned (Ga, Mn)As structures are addressed. First we focus on narrow
stripes. The four-fold symmetry of the reference sample shown in Fig.20b changes
into a pronounced two-fold symmetry when the (Ga, Mn)As ﬁlm is patterned into a
narrow stripe with a width of a few hundred nm (Fig.21a). As the lattice can relax
partially only along the side of the stripe for all three orientations of the stripes
([100], [010], [110]) the easy axis always coincides with the long axis of the stripe;
in agreement with earlier studies using SQUID and magneto-transport measurements
[102]. From these measurements we estimate the magnitude of the strain induced
anisotropy KU = 1.8×103 J
m3 for the 400nm wide stripe. For narrow stripes (below
a width of 500nm) the induced anisotropy saturates since the strain can be fully
relaxed across the stripe width. These results clearly demonstrate that the magnitude
of the induced uniaxial anisotropy can be well adjusted by using stripe widths ranging
between 500nm and 1.5 μm.
In the following disk-shaped elements are addressed. The angular dependence of
the resonance ﬁelds for a disk with a large diameter (d = 10 μm, black symbols) and
a small diameter (d = 1.5 μm, red symbols) is shown in Fig.22a. The experimental
data for the 10 μm-diameter disk were obtained at the disk center where the strain
40.
76 M. Farle et al.
(a) (b)
Fig. 21 Resonance ﬁeld as a function of the external ﬁeld angle ϕH for stripes patterned along
different crystallographic axes (a) and different stripe width w (b). All data was obtained at
f = 7.2GHz and T = 7K. The solid lines are ﬁts to the experimental data. From [101]
relaxation is almost zero. It should be emphasized that for a narrow rectangular
structure the strain can only relax in one direction giving rise to a strong uniaxial
anisotropy (Fig.21a). For a disk-shaped element we expect isotropic strain relaxation.
For this reason the in-plane anisotropies K2 and K4 should remain constant while
the strain-induced perpendicular anisotropy K2⊥ should be reduced. This reduction
is indeed observed (Fig.22a) as the resonance ﬁelds are only shifted to higher ﬁeld
values. The ﬁts to the experimental data show that K2 and K4 remain almost
constant while K2⊥ is reduced by approximately 20% for the disk with 1.5 μm
diameter.
Finally we demonstrate the ability to visualize the local variations of the mag-
netic anisotropies for both the disk-shaped and the rectangular (Ga, Mn)As structures.
Figure22c–e show spatially resolved images of the Kerr signal obtained at a ﬁxed
excitation frequency f and applied ﬁeld H. One ﬁnds laterally isotropic strain relax-
ation (indicated by the thick arrows in Fig.22b). Furthermore one can distinguish
two regions as illustrated in the ﬁgures: (i) the boundary of the structure where the
strain relaxation takes place and a strong uniaxial strain induced magnetic anisotropy
can be expected. And (ii) the central region of the structure where the (Ga, Mn)As
Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.
Be the first to comment